|Implantation of silicon dioxide-based nanocrystalline hydroxyapatite and pure phase beta-tricalciumphosphate bone substitute granules in caprine muscle tissue does not induce new bone formation.|
|Jump to Full Text|
|PMID: 23286366 Owner: NLM Status: Publisher|
|ABSTRACT: BACKGROUND: Osteoinductive bone substitutes are defined by their ability to induce new bone formation even at heterotopic implantation sites. The present study was designed to analyze the potential osteoinductivity of two different bone substitute materials in caprine muscle tissue.Materials and methods: One gram each of either a porous beta-tricalcium phosphate (beta-TCP) or an hydroxyapatite/silicon dioxide (HA/SiO2)-based nanocrystalline bone substitute material was implanted in several muscle pouches of goats. The biomaterials were explanted at 29, 91 and 181 days after implantation. Conventional histology and special histochemical stains were performed to detect osteoblast precursor cells as well as mineralized and unmineralized bone matrix. RESULTS: Both materials underwent cellular degradation in which tartrate-resistant acid phosphatase (TRAP)-positive osteoclast-like cells and TRAP-negative multinucleated giant cells were involved. The Ss-TCP was completely resorbed within the observation period, whereas some granules of the HA-groups were still detectable after 180 days. Neither osteoblasts, osteoblast precursor cells nor extracellular bone matrix were found within the implantation bed of any of the analyzed biomaterials at any of the observed time points. CONCLUSIONS: This study showed that Ss-TCP underwent a faster degradation than the HA-based material. The lack of osteoinductivity for both materials might be due to their granular shape, as osteoinductivity in goat muscle has been mainly attributed to cylindrical or disc-shaped bone substitute materials. This hypothesis however requires further investigation to systematically analyze various materials with comparable characteristics in the same experimental setting.|
|Shahram Ghanaati; Samuel E Udeabor; Mike Barbeck; Ines Willershausen; Oliver Kuenzel; Robert A Sader; C James Kirkpatrick|
Related Documents :
|8736026 - Calorimetric characterization of the formation of acrylic type bone cements.
24688566 - The effect of shape, length and diameter of implants on primary stability based on reso...
18681936 - The effects of repeated heat-pressing on properties of pressable glass-ceramics.
24480086 - Effect of bulk/incremental fill on internal gap formation of bulk-fill composites.
|Type: JOURNAL ARTICLE Date: 2013-1-4|
|Title: Head & face medicine Volume: 9 ISSN: 1746-160X ISO Abbreviation: Head Face Med Publication Date: 2013 Jan|
|Created Date: 2013-1-4 Completed Date: - Revised Date: -|
Medline Journal Info:
|Nlm Unique ID: 101245792 Medline TA: Head Face Med Country: -|
|Languages: ENG Pagination: 1 Citation Subset: -|
|APA/MLA Format Download EndNote Download BibTex|
Journal ID (nlm-ta): Head Face Med
Journal ID (iso-abbrev): Head Face Med
Publisher: BioMed Central
Copyright ©2013 Ghanaati et al.; licensee BioMed Central Ltd.
Received Day: 14 Month: 10 Year: 2012
Accepted Day: 10 Month: 12 Year: 2012
collection publication date: Year: 2013
Electronic publication date: Day: 4 Month: 1 Year: 2013
Volume: 9First Page: 1 Last Page: 1
PubMed Id: 23286366
Publisher Id: 1746-160X-9-1
|Implantation of silicon dioxide-based nanocrystalline hydroxyapatite and pure phase beta-tricalciumphosphate bone substitute granules in caprine muscle tissue does not induce new bone formation|
|Shahram Ghanaati12||Email: firstname.lastname@example.org|
|Samuel E Udeabor2||Email: email@example.com|
|Mike Barbeck1||Email: firstname.lastname@example.org|
|Ines Willershausen3||Email: email@example.com|
|Oliver Kuenzel1||Email: firstname.lastname@example.org|
|Robert A Sader2||Email: Robert.Sader@kgu.de|
|C James Kirkpatrick1||Email: email@example.com|
1Institute of Pathology, REPAIR-Lab, Johannes Gutenberg University Mainz, Langenbeckstrasse 1, Mainz, 55101, Germany
2Department for Oral, Cranio-Maxillofacial and Facial Plastic Surgery, Medical Center of the Goethe University Frankfurt, Frankfurt am Main, Germany
3Department for Operative Dentistry, Johannes Gutenberg University Mainz, Mainz, Germany
The search continues for an “ideal” bone substitute for the support, augmentation or replacement of bony tissue defects. Among other properties, these bone substitutes should ideally possess osteoconductivity, osteoinductivity and osteogenicity. Despite the increase in the number of surgical procedures that require bone grafts, there is still no ideal bone graft substitute . Although autografts are the gold standard that all other alternatives must meet or exceed, they have significant limitations, including donor site morbidity, inadequate tissue quantity, inappropriate forms [2,3] and sometimes the need for general anesthesia for their harvest [4,5]. These limitations have prompted increasing interest in alternative bone grafts. Allografts may be cancellous, cortical or a combination of these. Though they are attractive sources, several problems arise when using them, including the risk of disease transmission, immunogenicity  loss of biological and mechanical properties secondary to processing, increased cost, and lack of availability due to financial and religious-cultural concerns .
The drawbacks associated with natural bone grafts have led to the production of a large number of synthetic grafts. The latter are readily available, do not cause an antigenic response and can easily be tailored to the intended application. However, the biological performance of synthetic bone grafts in terms of initiation and support of bone growth is inferior to natural bone grafts . Their biological behaviour depends upon their chemical composition and physicochemical structure.4 A group of these synthetic biomaterials are termed osteoinductive biomaterials. These materials are potentially “intelligent” bone graft substitutes in that they are able to induce the in vivo environment to form bone . This also refers to their ability to stimulate and support the proliferation and differentiation of mesenchymal progenitor cells of the host tissue  when implanted in ectopic (i.e., extraskeletal) sites, together with the induction of bone formation [9,10]. Although the exact process of osteoinduction by biomaterials is still largely unknown, studies have shown that biomaterials need to meet very specific requirements in terms of macrostructure, microstructure and chemical composition in order to be osteoinductive [7,11].
The osteoinductive potential of NanoBone® (NB) hydroxyapatite/silicon dioxide (HA/SiO2)-based nanocrystalline bone substitute has been demonstrated in an in vivo study in mini pigs by Götz et al.. The authors reported both new bone formation and osteogenic differentiation which they claimed were better in the subcutaneous tissue than in the intramuscular implantation sites.
Our group has also been able to demonstrate in clinical trials the cellular pathway involved in NB degradation  and its osteoconductive capacity to promote sufficient new bone formation required for stable implant placement after three months .
The main aim of the present study was to investigate the osteoinductive potential of NB granules in goat intramuscular implantation sites in comparison with Cerasorb® a pure-phase beta tricalciumphosphate (ß-TCP) granules.
NanoBone® (Artoss, Rostock, Germany), a fully synthetic bone substitute granule, consists of hydroxyapatite crystallites with an average size of 60 nm in each crystallographic direction that are embedded in a matrix of silica gel. It is produced by a sol–gel-technique at temperatures below 700°C, avoiding sintering of the nanocrystalline hydroxyapatite . In the transition process from sol to gel, a loose connection of hydroxyapatite crystals with the SiO2 molecules takes place. This connection is responsible for a nanoporous structured bone substitute. The biomaterial is characterized by numerous open bonds, which are responsible for an internal surface of up to 84 m2/g in size. The pore size distribution within the silica gel ranges from 10 to 20 nm in diameter. Macroscopically, the fir cone-shaped NanoBone® granules possess an average length of 2 mm and an average diameter of 0.6 mm with a porosity of 60% - 80%.
The details of the synthesis of pure phase β-TCP and the fabrication of Cerasorb® M (Curasan, Kleinostheim, Germany) are described elsewhere . Briefly, pure phase β-tricalcium phosphate was synthesized by a solid-state reaction. After crushing and sieving a portion (< 63 μm) of the generated material, the ceramic particles were mixed with an organic porogen and pressed to rods. During a second sintering step (≥ 1000°C) the porogen disappeared. The resulting ceramic was highly porous with macropores of about 50–500 μm interconnected by micropores. After crushing the porous rods to splint granulates, the desired granulate sizes were reached by sieving. Finally Cerasorb® M was sterilized by gamma irradiation.
This study was performed in an accredited laboratory (RCC Ltd, Zelgliweg 1, 4452 Itlingen/Schwitzerland) in accordance with the Swiss Animal Protection Law under license (no. BL338) and by following internationally recognised guidelines. Six female goats (Capra hircus, Olsberg, Switzerland) were kept in agricultural animal husbandry in group housing of 100 square meters for six animals. Straw bedding was provided. Standard goat maintenance diet (Landi Jungfrau AG, Switzerland) was presented twice daily with water ad libitum. The animals were allocated into three groups of two animals each for the following time points: 28, 91 and 181 days.
Bone induction in ectopic tissue was analyzed by implanting the biomaterial in muscle pouches of the right Musculus longissimus dorsi (M. long. dorsi) and Musculus biceps femoris (M. biceps femoris). In each animal, one muscle pouch was operated without biomaterial implantation for the above mentioned time points (sham operation). These empty muscle pouches were used to classify the inflammatory response related to the operation in the absence of biomaterial implantation.
After medication with propofol at a dose sufficient to ensure appropriate induction of anesthesia (5–7 mg/kg i.v.), the level of anesthesia was maintained by means of isoflurane/oxygen via face-mask. Prior to surgery, the respective sites were shaved and disinfected with a standard of iodine/povidone (Betadine®) solution. Four to five muscle pouches per animal, either in the M. longissimus dorsi or M. biceps femoris, were formed after skin incision and blunt preparation with surgical scissors of approximately 0.5 cm diameter. A small amount of the biomaterial, i.e. 1.0 g, was deployed using glass-weighing boats with spouts for reliable positioning of the granular material in the muscle pouches. The muscle pouches were then closed with a button seam, likewise the following layers and the skin. All work was performed under sterile conditions. Postoperative analgesia consisted of single intramuscular injections of Metamizol at doses of 20 mg/kg body weight. During the acclimatization and post-surgical observation periods, the animals were only transiently separated for the assessment of clinical signs and body weights.
The animals were anesthetized with a captive bolt pistol and sacrificed by exsanguination. Immediately after death, the implantation beds containing the biomaterials were explanted together with the surrounding muscle pouches and fixed in 4% formalin for 24 hours for further histological and immunohistochemical analysis. The implant sites of each of the six animals were cut into three segments of identical dimensions of 4 mm thickness according to previously described methods.16 The central segment of the intramuscular pocket containing the biomaterial was used to identify osteoclast-like cells by staining for tartrate-resistant acid phosphatase (TRAP) and for the identification of osteoid and/or bone matrix by Movat´s pentachrome and Sirius red staining according to previously described methods [13,17,18].
The tissue reactions to the granules in goat muscles were varied and are highlighted under separate headings below.
Within the implantation bed of the nanocrystalline hydroxyapatite, the surface of the granules was surrounded by multinucleated giant cells. The degradation of the biomaterial was initiated from the periphery of the material and continued for the duration of the study (Figure 1A-C). Accordingly, the size of the granules decreased from day 29 until day 181 after implantation (Figure 1A-C). The multinucleated giant cells within the implantation bed of this bone substitute were mostly TRAP-negative. However, a few TRAP-positive multinucleated giant cells were also located on the surface of the HA-based material (Figure 2A). At day 91, the HA granules were well integrated within the implantation bed. At day 181 after implantation, the granules were penetrated by fibrous tissue and phagocytic cells resulting in their breakdown and disintegration (Figure 2C). At no time within the observational period osteoblasts or bone-specific matrix could be identified via immunohistochemical staining methods in any implantation bed of this nanocrystalline bone substitute.
Within the implantation bed of the β-TCP-based bone substitute, all granules were well integrated. As early as day 28 after implantation, connective tissue fibers as well as phagocytic cells, such as macrophages and multinucleated giant cells, penetrated the center of the granules. Also at this time point, a progressive degradation of the material was visible, and small particles of the granules were incorporated into multinucleated giant cells (Figure 1D). The β-TCP-based granules were almost completely degraded at day 91 after implantation (Figure 1E). At this time point, the major part of the implantation bed was invaded by multinucleated giant cells, which contained small components of the granules within their cytosol. At day 181 after implantation, the β-TCP-based bone substitute material was totally degraded and only collagenous fibrous tissue with a few vessels remained (Figure 1F). Within the implantation bed, TRAP-positive multinucleated giant cells that were involved in the degradation of the biomaterial could be found. However, their number seemed to be higher within the implantation bed of the β-TCP-based bone substitute when compared with the implantation bed of the nanocrystalline material (Figure 2B). Neither osteoblasts nor bone-specific matrix was found in any of the implantation beds of this β-TCP-based bone substitute at any time point.
The present study demonstrated that the two bone substitute materials showed differences in the extent of multinucleated giant cell formation within their implantation beds. Multinucleated giant cells in the implantation bed of the β-TCP-based bone substitute were mostly TRAP-positive, whereas only a few TRAP-positive giant cells were located on the surface of NB. The higher presence of multinucleated giant cells, especially the TRAP-positive subpopulation within the implantation bed of β-TCP, reflects the influence of the chemical composition of this bone substitute on the expression of the degrading enzyme tartrate-resistant acid phosphatase [19,20]. Accordingly, the high presence of multinucleated giant cells might be related to the composition of the used β-TCP and might be, in addition to dissolution, a reason for its comparably faster degradation [19,20]. Multinucleated giant cells are known to originate from mononuclear phagocytic cells such as macrophages [21-23] and their presence reflects the foreign body reaction, which is described for such biomaterials [13,20,24]. Thus, gene expression of degrading enzymes like TRAP is dependent on the characteristics of the biomaterial [21,22,25].
The degradation pattern which was observed for NB in this study is similar to what our group had previously reported following material implantation in subcutaneous tissue of Wistar rats . This material underwent a more continuous degradation over time, and the breakdown of the granules into particles took place at later stages of the study.
The control over the degradation rate of a biomaterial is an essential aspect for its contribution to bone remodeling. Studies investigating the osteoinductive properties of macroporous calcium phosphate cements postulated that fast biomaterial degradation may have a negative influence on its osteoinductive characteristics . Thus, a fast degradation will result in a connective tissue influx, which might inhibit bone regeneration in the respective defect . However, it remains unclear to what extent this connective tissue influx into a bone defect as a result of biomaterial degradation might undergo differentiation into bone over time. Therefore, the activity of degrading cells could be controlled by the physicochemical characteristics of the material, as shown by the two analyzed materials.
In this study, we have studied the potential osteoinductivity of the two bone substitute materials by means of histological and histochemical staining methods. Throughout the study period, no osteoblasts or bone-specific matrices could be found in any implantation bed of the used NB granules. These data are in accordance with previous studies, which also failed to show osteoinductive properties of HA-based bone substitutes within goat muscle when compared to various forms of porous biphasic calcium phosphates (BCP) . However, it must be mentioned that the other authors used cylindrically-shaped calcium phosphate ceramics  and not granules as in the present study. Despite the presence of micro- and nanopores, NB in its granular form within caprine muscle probably did not induce sufficient mineral ion influx and protein-related surface modifications, which are suggested as a requirement to trigger osteoinduction [27-29]. On the other hand, another in vivo study in mini pigs reported a marked osteoinduction within subcutaneous as well as muscle implantation sites induced by the very same NB-granules . Thus, we assume that the lack of osteoinductivity of NB in the present study could be explained on the basis of its application form, i.e. granules and the animal species.
It is noteworthy that β-TCP granules, which were used as controls in the present study, stimulated neither osteoblasts nor bone-specific matrices in any of the implantation beds throughout the observational period. The failure of β-TCP to induce ectopic bone formation when applied as a single bone substitute material has also been previously described . In combination with bone marrow stromal cells , however, and along with hydroxyapatite as biphasic calcium phosphate ceramics [32-34], it has been shown to induce different degrees of osteoinductivity, even in ectopic tissues. With regard to objectivity, it has to be considered whether the used ß-TCP granules would have shown some osteoinductive properties, when implanted into the subcutaneous or muscle tissue of the mini-pig as was done for NB . Furthermore, it has to be emphasized that for ß-TCP, osteoinduction has been demonstrated in dogs [35,36]. However, the materials used for the dog study were of different morphology, namely either cylindrical or disc shape.
The reasons for lack of ectopic bone formation in the present study are not apparent. Despite the fact that the principle behind the process of osteoinduction is largely unknown, it is believed to be positively influenced by the chemical composition of biomaterials , their sintering temperature , material dissolution , macro- and microporosity [36-38], implant size and the applied animal model [34,39]. Besides these factors, inflammation itself might be an influencing factor for bone induction. The release of cytokines, which consequently lead to a higher circulation within the implantation bed, stimulate circulating stem cells to differentiate into osteoblastic cells . Accordingly, a better understanding of the degradation-related inflammatory response may contribute to better tailoring of bone substitute materials.
Based on the results of this study and the available literature, it is evident that ectopic bone formation is highly influenced by the chosen animal model, i.e. subcutaneous vs. intramuscular implantation sites, species, for example, goat vs. monkey, dog, mini-pig and sheep, as well as morphology, i.e. porous granules vs. solid structures such as cylindrical or disc-shaped materials. The granular form seems to be an influential parameter to a higher extent than previously assumed. These differences might be the reason why the implantation of the NB-granules led to ectopic bone formation in the subcutaneous and the muscle tissue of mini-pigs , while no osteoinductive capacity was observed when the same granules were implanted into caprine muscle.
These findings notwithstanding, our group and other groups have been able to show appreciable success with the clinical application of both bone substitute materials used here [13,14,40-42]. Despite their potential lack of de novo bone formation in an ectopic large animal model, they are still very relevant as viable alternatives to autografts as the search for the “ideal” bone substitute continues. The present study demonstrates that success nor failure of ectopic bone formation induced by biomaterials should not be over interpreted. The primary focus should be placed on the clinical outcome e.g. implantation and on the adaptation of the applied materials to the patient’s individual needs.
The present study showed that ß-TCP granules induced more TRAP-positive multinucleated giant cell inflammatory reaction compared to NB granules. Consequently, the former underwent faster degradation. It has to be elucidated, whether the detected multinucleated giant cells within the implantation bed of the used materials are foreign body giant cells or osteoclasts. The former are involved in foreign body reactions, while the latter are known to induce the differentiation of mesenchymal stem cells into osteoblasts. The understanding of the molecular mechanism of the multinucleated giant cells involved in calcium phosphate ceramic degradation is of high relevance, especially since this knowledge might help to understand the interaction of inflammation and osteoinduction. Neither osteoblasts nor newly formed bone were detected in any of the implantation beds of the two materials at any time point during the study. The lack of osteoinduction observed here especially in the case of NB might be a result of its application form, i.e. granules and the animal model used. Osteoinduction was previously reported in goat muscle tissue related to cylindrical or disc-shaped calcium phosphate ceramics and not granules. On the other hand it has been documented that osteoinduction occurred for NB in granular form in the muscle tissue of mini-pigs. Accordingly, the question arises which material characteristics and which micro-environment are required to induce osteoinduction in calcium phosphate ceramic granules. It should however be noted that the lack of osteoinductivity in ectopic tissue in an animal model does not necessarily predict the potential of these materials to induce de novo bone formation in humans. Indeed clinically, the two materials investigated in this study have proven to be suitable for human bone regeneration.
Hereby we confirm that this article is not reviewing by other journals. The authors declare that they have no competing of interests.
SG, SEU, MB and OK carried out the in vivo experiments, histological analyses as well as the histological imaging. SG, SEU, MB, IW, OK, RAS and CJK were involved in writing of the manuscript.
The authors would like to thank Mrs. Ulrike Hilbig for her expert assistance in histological preparation. The data of this work represent parts of the data of the medical thesis of Mr. Oliver Kuenzel, Johannes Gutenberg University of Mainz.
|Parikh SN,Bone grafts substitutes: past, present, futureJ Postgrad MedYear: 20024814214812215702|
|Banwart JC,Asher MA,Hassanein RS,Iliac crest bone graft harvest donor site morbidity: a statistical evaluationSpineYear: 1995201055106010.1097/00007632-199505000-000127631235|
|Cowley SP,Anderson LD,Hernias through donor sites for iliac-bone graftsJ Bone Joint Surg AmYear: 198365102310256885861|
|Finkemeier CG,Bone-grafting and bone graft substitutesJ Bone Joint SurgYear: 20028445446411886919|
|Younger EM,Chapman MW,Morbidity at bone graft donor sitesJ Orthop TraumaYear: 1989319219510.1097/00005131-198909000-000022809818|
|Friedlaender GE,Immune responses to osteochondral allografts. Current knowledge and future directionsClin Orthop Relat ResYear: 198317458686339143|
|Habibovic P,de Groot K,Osteoinductive biomaterials – properties and relevance in bone repairJ Tissue Eng Regen MedYear: 20071253210.1002/term.518038389|
|Traianedes K,Russell JL,Edwards JT,Stubbs HA,Shanahan IR,Knaack D,Donor age and gender effects on osteoinductivity of demineralised bone matrixJ Biomed Mater Res B Appl BiomaterYear: 200470212915199579|
|Habibovic P,Yuan H,van den Doel M,Sees TM,van Blitterswijk CA,de Groot K,Relevance of osteoinductive biomaterials in critical-sized orthotopic defectJ Orthop ResYear: 20062486787610.1002/jor.2011516596652|
|Yao J,Li X,Bao C,Zhang C,Chen Z,Fan H,et al. Ectopic bone formation in adipose-derived stromal cell-seeded osteoinductive calcium phosphate scaffoldsJ Biomater ApplYear: 20102460762410.1177/088532820910429419386665|
|Habibovic P,Yuan H,van der Valk CM,Meijer G,van Blitterswijk CA,de Groot K,3D Microenvironment as essential element for osteoinduction by biomaterialsBiomaterialsYear: 2005263565357510.1016/j.biomaterials.2004.09.05615621247|
|Götz W,Lenz S,Reichert C,Henkel KO,Bienengräber V,Pernicka L,et al. A preliminary study in osteoinduction by a nano-crystalline hydroxyapatite in the mini pigFolia Histochem CytobiolYear: 20104858959621478102|
|Stübinger S,Ghanaati S,Orth C,Hilbig U,Saldamli B,Biesterfeld S,et al. Maxillary sinus grafting with a nano-structured biomaterial: preliminary clinical and histological resultsEur Surg ResYear: 20094214314910.1159/00019721519176966|
|Ghanaati S,Barbeck M,Willershausen I,Thimm B,Stuebinger S,Korzinskas T,et al. Nanocrystalline hydroxyapatite bone substitute leads to sufficient bone tissue formation already after 3 months: histological and histomorphometrical analysis 3 and 6 months following human sinus cavity augmentationClin Implant Dent Relat ResYear: 201210.1111/j.1708-8208.2011.00433.x|
|Gerber T,Holzhueter G,Goetz W,Bienengraeber V,Henkel KO,Rumpel E,Nanostructuring of biomaterials - a pathway to bone grafting substituteEur J TraumaYear: 20063213214010.1007/s00068-006-6046-9|
|Peters F,Reif D,Functional materials for bone regeneration from beta- tricalcium phosphatMater WerkstYear: 20043520320710.1002/mawe.200400735|
|Ghanaati S,Webber MJ,Unger RE,Orth C,Hulvat JF,Kiehna SE,Dynamic in vivo biocompatibility of angiogenic peptide amphiphile nanofibersBiomaterialsYear: 2009306202621210.1016/j.biomaterials.2009.07.06319683342|
|Ghanaati SM,Thimm BW,Unger RE,Orth C,Kohler T,Barbeck M,et al. Collagen-embedded hydroxylapatite-beta-tricalcium phosphate-silicon dioxide bone substitute granules assist rapid vascularization and promote cell growthBiomed MaterYear: 201052500410.1088/1748-6041/5/2/02500420208127|
|Barrère F,van Blitterswijk CA,de Groot K,Bone regeneration: molecular and cellular interactions with calcium phosphate ceramicsInt J NanomedicineYear: 20061331733217717972|
|Ghanaati S,Barbeck M,Detsch R,Deisinger U,Hilbig U,Rausch V,et al. The chemical composition of synthetic bone substitutes influences tissue reactions in vivo: histological and histomorphometrical analysis of the cellular inflammatory response to hydroxyapatite, beta-tricalcium phosphate and biphasic calcium phosphate ceramicsBiomed MaterYear: 20127101500510.1088/1748-6041/7/1/01500522287541|
|Anderson JM,Biological responses to materialsAnnu Rev Mater ResYear: 2001318111010.1146/annurev.matsci.31.1.81|
|Anderson JM,Rodriguez A,Chang DT,Foreign body reaction to biomaterialsSemin ImmunolYear: 2008208610010.1016/j.smim.2007.11.00418162407|
|Brodbeck WG,Anderson JM,Giant cell formation and functionCurr Opin HematolYear: 200916535710.1097/MOH.0b013e32831ac52e19057205|
|Ghanaati S,Orth C,Barbeck M,Willershausen I,Thimm BW,Booms P,et al. Histological and histomorphometrical analysis of a silica matrix embedded nanocrystalline hydroxyapatite bone substitute using the subcutaneous implantation model in wistar ratsBiomed MaterYear: 2012503500520460687|
|Webster TJ,Ergun CD,Siegel RW,Bizios R,Enhanced functions of osteoclast-like cells on nanophase ceramicsBiomaterialsYear: 2001221327133310.1016/S0142-9612(00)00285-411336305|
|Henkel KO,Gerber T,Lenz S,Gundlach KK,Bienengräber V,Macroscopical, histological, and morphometric studies of porous bone-replacement materials in minipigs 8 months after implantationOral Surg Oral Med Oral Pathol Oral Radiol EndodYear: 200610260661310.1016/j.tripleo.2005.10.03417052636|
|Geesink RG,de Groot K,Klein CP,Bonding of bone to apatite-coated implantsJ Bone Joint Surg BrYear: 1988701111711122|
|Hanawa T,Kamiura Y,Yamamoto S,Kohgo T,Amemiya A,Ukai H,et al. Early bone formation around calcium-ion-implanted titanium inserted into rat tibiaJ Biomed Mater ResYear: 19973613113610.1002/(SICI)1097-4636(199707)36:1<131::AID-JBM16>3.0.CO;2-L9212398|
|Kay JF,Cook SD,Geesink RGT, Manley MTBiological profile of calcium phosphate coatingsHydroxylapatite coatings in orthopaedic surgeryYear: 1993New-York, USA: Raven Press Ltd89106|
|Eid K,Zelicof S,Perona BP,Sledge CB,Glowacki J,Tissue reactions to particles of bone-substitute materials in intraosseous and heterotopic sites in rats: discrimination of osteoinduction, osteocompatibility, and inflammationJ Orthop ResYear: 20011996296910.1016/S0736-0266(00)00080-211562148|
|Orii H,Sotome S,Chen J,Wang J,Shinomiya K,Beta-tricalcium phosphate (beta-TCP) graft combined with bone marrow stromal cells (MSCs) for posterolateral spine fusionJ Med Dent SciYear: 200552515715868741|
|Ghanaati S,Barbeck M,Orth C,Willershausen I,Thimm BW,Hoffmann C,et al. Influence of beta-tricalcium phosphate granule size and morphology on tissue reaction in vivoActa BiomaterYear: 201064476448710.1016/j.actbio.2010.07.00620624495|
|Kurashina K,Kurita H,Wu Q,Ohtsuka A,Kobayashi H,Ectopic ostegenesis with biphasic ceramics of hydroxyapatite and tricalcium phosphates in rabbitsBiomaterialsYear: 20022340741210.1016/S0142-9612(01)00119-311761160|
|Le Nihouannen D,Daculsi G,Saffarzadeh A,Gauthier O,Delplace S,Pilet P,et al. Ectopic bone formation by microporous calcium phosphate ceramic particles in sheep musclesBoneYear: 2005361086109310.1016/j.bone.2005.02.01715869915|
|Yuan H,Yang Z,Li Y,Zhang X,de Bruijn JD,de Groot K,Osteoinduction by calcium phosphate biomaterialsJ Mater Sci Mater MedYear: 1998972372615348929|
|Yuan H,de Bruijn JD,Li Y,Feng J,Yang Z,De Groot K,et al. Bone formation induced by calcium phosphate ceramics in soft tissue of dogs: a comparative study between porous alpha-TCP and beta-TCPJ Mater Sci Mater MedYear: 200112171310.1023/A:102679261566515348371|
|Habibovic P,Sees TM,van den Doel MA,van Blitterswijk CA,de Groot K,Osteoinduction by biomaterials physicochemical and structural influencesJ Biomed Mater Res AYear: 20067774776216557498|
|Gosain AK,Song L,Riordan P,Amarante MT,Nagy PG,Wilson CR,et al. A 1-year study of osteoinduction in hydroxyapatite-derived biomaterials in an adult sheep model: part IPlast Reconstr SurgYear: 200210961963010.1097/00006534-200202000-0003211818845|
|Ripamonti U,Osteoinduction in porous hydroxyapatite implanted in heterotopic sites of different animal modelsBiomaterialsYear: 199617313510.1016/0142-9612(96)80752-68962945|
|Zerbo IR,Zijderveld SA,de Boer A,Bronckers AL,de Lange G,ten Bruggenkate CM,et al. Histomorphometry of human sinus floor augmentation using a porous beta-tricalcium phosphate: a prospective studyClin Oral Implants ResYear: 20041572473210.1111/j.1600-0501.2004.01055.x15533134|
|Zerbo IR,Bronckers AL,de Lange GL,van Beek GJ,Burger EH,Histology of human alveolar bone regeneration with a porous tricalcium phosphate. A report of two casesClin Oral Implants ResYear: 20011237938410.1034/j.1600-0501.2001.012004379.x11488868|
|Canullo L,Dellavia C,Sinus lift using a nanocrystalline hydroxyapatite silica gel in severely resorbed maxillae: histological preliminary studyClin Implant Dent Relat ResYear: 200911Suppl 1713|
Keywords: Osteoinduction, Cerasorb, NanoBone, Nanocrystalline, ß-tricalciumphosphate, Hydroxyapatite, Ectopic bone formation.
Previous Document: Enantioselective Synthesis of 2-Arylbicyclo[1.1.0]butane Carboxylates.
Next Document: Design and Implementation of Two-Dimensional Polymer Adsorption Models: Evaluating the Stability of ...